 real ($\sigma_1$) and imaginary ($\sigma_2$) THz conductivity of one particular LSCO film (x=0.095, $T_c$=23.5K) out of a large series we have recently studied [@Bilbro11a]. At high temperature $\sigma_1$ is fairly constant in frequency. As the temperature is lowered, $\sigma_1$ increases, develops a frequency dependence near $T_c$, and then decreases as spectral weight is shifted into a delta function at zero frequency. The $\sigma_2$ vs. frequency data in Fig. 1(b) show a small imaginary part of the conductivity at high temperatures, which is enhanced dramatically as temperature is reduced near $T_c$. At the lowest displayed temperatures $\sigma_2$ shows the 1/$\omega$ dependence expected for the superfluid response of a superconductor. While the low and high-temperature limits are easily understood, we are most interested in the fluctuation regime near $T_c$.

The enhancement of the conductivity in this fluctuation regime is more clear in Fig. 1(c) and (d), where we plot $\sigma_1$ and $\sigma_2$ vs. temperature. One can see clearly the slow increase and subsequent decrease in $\sigma_1$ as temperature is lowered below $T_c$. At low frequency there is a well-defined peak around $T_c$. The location of this peak shifts to lower temperature as frequency is reduced corresponding to the slowing down of fluctuations as the temperature decreases. Above $T_c$, we see a sudden onset in $\sigma_2$ at a temperature $T$ $\approx$ 30K. In earlier work, we found that the second derivative with respect to temperature of the quantity $\omega\sigma_2$ (which is related to the phase stiffness) showed a clear and dramatic onset from a near-zero high-temperature signal [@Bilbro11a]. We denoted this temperature as $T_o$, and defined it as the onset of superconducting fluctuations in the charge conductivity (for this film $T_o\approx$ 31K). Note that there is no sign of conductivity enhancement at the high temperatures of the Nernst or diamagnetism onset [@Xu00a; @Wang05a; @Li10a].

![(a) Magnitude of the conductivity ($|\sigma|$) as function of temperature. The filled region is a fit of the normal state background conductivity at 300 GHz
real ($ \sigma_1 $) and imaginary ($ \sigma_2 $) THz conductivity of one especial LSCO movie (x=0.095, $ T_c$=23.5 K) out of a large serial we have recently studied [ @Bilbro11a ]. At gamey temperature $ \sigma_1 $ is fairly constant in frequency. As the temperature is frown, $ \sigma_1 $ increases, develops a frequency addiction near $ T_c$, and then decrease as spectral weight unit is shifted into a delta function at zero frequency. The $ \sigma_2 $ vs. frequency datum in Fig. 1(b) show a small imaginary part of the conductivity at high temperatures, which is enhance dramatically as temperature is reduced near $ T_c$. At the lowest displayed temperature $ \sigma_2 $ shows the 1/$\omega$ dependence expected for the superfluid response of a superconductor. While the abject and high - temperature limits are easily understood, we are most concerned in the fluctuation regime near $ T_c$. 

 The enhancement of the conductivity in this fluctuation regime is more clear in Fig. 1(c) and (d), where we diagram $ \sigma_1 $ and $ \sigma_2 $ vs. temperature. One can see clearly the slow increase and subsequent decrease in $ \sigma_1 $ as temperature is lowered below $ T_c$. At low frequency there is a well - defined peak around $ T_c$. The location of this extremum shifts to lower temperature as frequency is reduce represent to the slowing down of fluctuations as the temperature decrease. Above $ T_c$, we see a sudden onset in $ \sigma_2 $ at a temperature $ T$ $ \approx$ 30K. In earlier work, we detect that the second derivative with respect to temperature of the quantity $ \omega\sigma_2 $ (which is related to the phase severity) showed a clear and dramatic onset from a near - zero eminent - temperature signal [ @Bilbro11a ]. We denoted this temperature as $ T_o$, and specify it as the onset of superconducting fluctuations in the charge conductivity (for this film $ T_o\approx$ 31 K). notice that there is no sign of conductivity enhancement at the high temperatures of the Nernst or diamagnetism onset [ @Xu00a; @Wang05a; @Li10a ]. 

! [ (a) Magnitude of the conductivity ($ |\sigma|$) as function of temperature. The filled region is a burst of the normal state backdrop conductivity at 300 GHz
 rewl ($\sigma_1$) and imaginary ($\slgma_2$) THz conductncity oh one pzrticulaf LSCO film (x=0.095, $T_c$=23.5K) out of a lerge seritf we have recently studied [@Hilbro11a]. Qt hmgh temperature $\sigma_1$ is fairlg convvant in frequengy. As the tamperature is nodexed, $\sigma_1$ increases, develops a frequqncy delejdence near $T_c$, and ehen decreases as spectral weight is sgifted pnto a delta funcyion at zero frequency. The $\sigla_2$ vs. frequency daha in Fig. 1(b) shor a small imaeinary paru mf the consuctivity at high temperatures, dhich is enhancgb drwkatically aw temierature is rccuced tear $T_c$. At the lowest divplqyed temperatures $\sigka_2$ shows the 1/$\omega$ dependenwe expected for the syperfnuid resoinsd or e shpercojdurtor. While fhe low and high-temperature likiew are easily hnderseojd, we are most interested in the fluctudtikn regime near $T_c$.

The enyancement of the condoctivity ig this fluctuation regime is more clear in Fig. 1(c) dnd (d), dhexc dw olot $\sigma_1$ and $\sigma_2$ vs. temperature. One can sqs vlvarly the slow ingrease and subsequrnh cgcrease in $\sigoa_1$ as csmlerature is loweref below $T_c$. Ar low frezuenvy there is a well-defined pwak around $T_b$. Thw location of this peak shiftr to lowet temperature as frequeucy is reduced cogrespondihe to the slowing doen of flucujations as the teiperature decxeases. Acove $T_c$, we see a sudfen okvet in $\sigma_2$ at a hempetature $T$ $\approx$ 30N. In earlier work, we found that the second detivdtine with rzspect to temperatuwe of the quanjity $\omegc\sigma_2$ (which is gelated tm the phase stiffness) shmaed a clear end dramaeic inser from x near-zero high-yemperatuge sigbal [@Bilbro11a]. We denptea this temperatuxt aw $T_o$, and definec ig af nhe ogvet of superwondjctkmg fljctuations ln ghe vharge conductivity (xor fhis film $T_o\approx$ 31K). Note thqt there is no sign og conductivity enhwncemxnt at the nigr temperatures of the Nernst od diamagnftifm onset [@Xu00a; @Wann05a; @Ly10a].

![(a) Magnitbde of the conductivity ($|\sigma|$) as functioi of temperature. The fioled region is a fij on the normal statq backgrognd conductivity at 300 GHz
real ($\sigma_1$) and imaginary ($\sigma_2$) THz conductivity particular film (x=0.095, out of a studied At high temperature is fairly constant frequency. As the temperature is lowered, increases, develops a frequency dependence near $T_c$, and then decreases as spectral weight shifted into a delta function at zero frequency. The $\sigma_2$ vs. frequency data Fig. show small part of the conductivity at high temperatures, which is enhanced dramatically as temperature is reduced near At the lowest displayed temperatures $\sigma_2$ shows the dependence expected for the response of a superconductor. While low high-temperature limits easily we most interested in fluctuation regime near $T_c$. The enhancement of the conductivity in this fluctuation regime is more clear in 1(c) and we plot and vs. One can see slow increase and subsequent decrease in is lowered below $T_c$. At low frequency there a well-defined around $T_c$. The location of this shifts to lower temperature as frequency is reduced to the slowing down of fluctuations as the temperature decreases. Above $T_c$, we see a in $\sigma_2$ at a $T$ $\approx$ 30K. earlier we that second derivative respect to temperature of the quantity $\omega\sigma_2$ (which is related to phase stiffness) showed a clear and dramatic onset from a signal We denoted this as $T_o$, and defined as onset of superconducting fluctuations charge (for 31K). that is no sign of enhancement at the high temperatures the Nernst or diamagnetism Magnitude of the conductivity ($|\sigma|$) as function of The filled region is a fit of normal state background conductivity at 300 GHz
 real ($\sigma_1$) and imaginary ($\sigmA_2$) THz conducTivitY of One PaRticUlar lSCO film (x=0.095, $T_c$=23.5K) ouT Of a lArge series we have recentLy stuDiED [@BilBRo11A]. At hiGh tempeRAtURE $\siGmA_1$ iS faIrLY cOnstaNt iN frequeNcy. As the teMpeRaTure is lowereD, $\SiGma_1$ increasEs, dEvelops a freqUenCy depeNdEncE Near $T_C$, anD then DecreaSEs as spEctral weiGhT Is shifTEd into a DELtA funCtion at zero frequeNCy. tHe $\sigma_2$ vs. frequEncy daTa IN FIG. 1(B) shOw a Small imagiNaRy parT Of the coNDuCTIVitY At high temperaTures, which iS EnhAnced dRaMatICally aS tempErATurE is reduced nEar $T_C$. At the lowEst disPLayed teMPeraturEs $\sigmA_2$ shOws The 1/$\oMEgA$ dEpeNdENce EXpEctED foR the supeRfLuId resPonsE OF A SupeRcoNducTor. WhIle the low and hIgh-TempERatUre liMits aRe eaSiLy undErstooD, we arE mOst interested in The fLuctuatioN reGiMe nEaR $T_c$.

ThE EnhancEmeNt oF the conDuctiviTY in ThIS FLuCtuation regime is moRe CLEaR in Fig. 1(c) aNd (d), wheRE wE pLOt $\sigma_1$ aNd $\SigMa_2$ vs. TEMperaTure. oNe Can see clEarly tHE sLoW increaSe And subSeQueNt dEcreaSE in $\sIgma_1$ as TemperatUre is LOwered below $T_c$. AT Low frequency tHErE IS a WEll-dEfiNed peak arouNd $T_c$. tHe loCatiON oF thIS peak ShiftS tO LoWEr temperature as freqUeNcy is rEduceD correspondinG to the slowING Down of flUctuATiONs as the temperaTure dEcreases. AbOVe $T_c$, we seE a sudDen onset In $\sigma_2$ at A TEmperatuRe $T$ $\AppRox$ 30k. In EARlIer work, we founD THat tHe Second dEriVative wIth ResPecT to TeMperature Of the quaNtItY $\oMeGa\sIgma_2$ (wHIch is relAtEd tO tHe pHase sTIffnesS) showEd a cLeAr ANd dRamatic ONsET From A nEaR-zerO hiGh-TempeRatuRE siGnal [@BilBro11a]. We denOteD This TeMpErature As $T_o$, and defineD iT as the onseT oF suPerconDUCting fluCtuations in the charge conDUctivitY (foR this Film $t_o\approx$ 31K). notE that tHerE Is no siGn of coNductIvIty ENHanceMENt At tHe High temperATUreS of thE NErnsT or diamAgnetism onset [@Xu00a; @WaNG05a; @LI10a].

![(a) Magnitude oF thE conDUCtIviTY ($|\sIGma|$) As FUncTIOn of temperature. the filled rEgIOn Is a fit of thE NorMaL state bAckgrouNd conDUctivitY at 300 GHz
 real ($\sigma_1$) and ima ginary ($\ sigma _2$ ) T Hz  con duct ivity of one p a rtic ular LSCO film (x=0.09 5, $T _c $ =23. 5 K)  outof a la r ge s eri es  w e h av e  r ecent lystudied  [@Bilbro1 1a] .At high temp e ra ture $\sig ma_ 1$ is fairly  co nstant  i n f r equen cy.  As t he tem p eratur e is lowe re d , $\si g ma_1$ i n c re ases , develops a freq u en c y dependence n ear $T _c $ ,a n d t hen  decreases  a s spe c tral we i gh t i s s h ifted into adelta funct i onat zer ofre q uency.  The$\ s igm a_2$ vs. fr eque ncy datain Fig .  1(b) s h ow a sm all im agi nar y pa r tof  th ec ond u ct ivi t y a t high t em pe ratur es,w h i c h is  en hanc ed dr amatically as  te mper a tur e isreduc ed n ea r $T_ c$. At  thelo west displayedtemp eratures$\s ig ma_ 2$  show s  the 1 /$\ ome ga$ dep endence exp ec t e d  f or the superfluidre s p on se of asuperc o nd uc t or. Whil ethe  low a nd hi gh-t e mp eraturelimits ar eeasilyun dersto od , w e a re mo s t in terest ed in th e flu c tuation regime near $T_c$.
T he e nh a ncem ent  of the con duct i vity  int hi s f l uctua tionre g im e  is more clear in F ig . 1(c)  and(d), where we  plot $\si g m a _1$ and$\si g ma _ 2$ vs. tempera ture.  One can s e e clearl y the  slow in crease an d subseque ntdec rea sei n  $ \sigma_1$ ast e mper at ure islow ered be low  $T _c$ . A tlow frequ ency the re  i sawel l-def i ned peak  a rou nd  $T _c$.T he loc ation  ofth is pea k shift s  t o lowe rte mper atu re  as f requ e ncy  is red uced corr esp o ndin gto  the sl owing down of  f luctuation sasthe te m p eraturedecreases. Above $T_c$, we seea s udden  ons et in $\s igm a_2$ a t a temper ature$T$ $ \a ppr o x $ 30K . In  ea rl ier work,w e  fo und t ha t th e secon d derivative withr esp ect to temper atu re o f th e q u an t ity  $ \ ome g a \sigma_2$ (whic h is relat ed to  the phase sti ff ness) s howed a  clea r  and dr amatic on set fromanear - z ero  high-temp eraturesignal [@ B ilbro 1 1a ]. We  de notedth istempe rature as$T_o$ , andde finedit as  t he onset  of superconducting flu ctuati ons i n t he charge  co n duc tivity (f or t his film $ T_o \ap prox$  31 K ). No te t h at  th e re is  nos ign of co n du cti v i ty  enhancemen t a t t he hi ght empera ture s of the Nernst o r  diamagnetismonse t [@X u00 a ; @W an g05a; @Li10a]. 

! [( a )  Magnitu de  of the con ductivit y( $|\si gma|$)  as fu nctiono f  t e mperat ure.  Th e filledreg io n  is a f it  o f  the n orma lstatebackgr o undc o nductivity at 30 0 GHz 
 real_($\sigma_1$) and_imaginary ($\sigma_2$) THz conductivity_of one_particular_LSCO film_(x=0.095,_$T_c$=23.5K) out of_a large series_we have recently studied_[@Bilbro11a]. At high_temperature_$\sigma_1$ is fairly constant in frequency. As the temperature is lowered, $\sigma_1$ increases, develops_a_frequency dependence_near_$T_c$,_and then decreases as spectral_weight is shifted into a_delta function_at zero frequency. The $\sigma_2$ vs. frequency data_in_Fig. 1(b) show_a small imaginary part of the conductivity at high_temperatures, which is enhanced dramatically as_temperature is reduced_near_$T_c$._At the lowest displayed_temperatures $\sigma_2$ shows the 1/$\omega$ dependence_expected for the superfluid response of_a superconductor. While the low and high-temperature_limits are easily understood, we are_most interested in the fluctuation_regime near_$T_c$.

The enhancement of the conductivity_in this fluctuation_regime is_more clear in_Fig. 1(c) and (d), where we_plot $\sigma_1$ and_$\sigma_2$ vs. temperature. One can see_clearly_the slow increase_and_subsequent_decrease in_$\sigma_1$ as temperature_is_lowered below_$T_c$._At low frequency there is a_well-defined_peak around $T_c$. The location of this_peak shifts to lower_temperature_as frequency is reduced_corresponding to the slowing down_of fluctuations as the temperature decreases._Above $T_c$,_we see_a sudden onset in $\sigma_2$ at a temperature $T$ $\approx$ 30K._In earlier work, we found that_the second derivative with_respect to_temperature_of the quantity_$\omega\sigma_2$_(which is_related to the phase stiffness) showed a_clear and_dramatic onset from a near-zero high-temperature_signal [@Bilbro11a]. We denoted_this_temperature as $T_o$, and defined it_as the onset of superconducting fluctuations_in the charge conductivity (for_this_film_$T_o\approx$ 31K). Note that there_is no sign of conductivity enhancement_at the high_temperatures of the Nernst or diamagnetism onset_[@Xu00a;_@Wang05a; @Li10a].

![(a) Magnitude of the conductivity_($|\sigma|$)_as function of temperature. The filled_region_is_a fit of the normal_state background conductivity at 300 GHz